### Redistribution of Solute during Cellular Solidiﬁcation of Single Phase Alloys

### Toshiro Owadano

*Kyushu Institute of Technology, Kitakyushu 804-8550, Japan

Computer simulation of the upward cellular solidiﬁcation of Al–Cu alloy was carried out considering the solidiﬁcation to be a reaction controlled by diﬀusion. In the simulation, direct solving method of diﬀerential equation was applied to the diﬀusion in solid and liquid in contact with each other during cooling. The results of simulation showed that the solute distribution in liquid groove ahead of the solid-liquid interface is parabola whose bottom zenith lies at cell boundary. This result, together with the negligible diﬀusion in solid, induced that Scheil’s equation is approximately applicable to the solute distribution in the solid cell after the solidiﬁcation. Numerical analysis of the simulated results induced also a general equation which expresses the parabolic relationship between cooling rate and the cell size. The validity of thus induced equation was veriﬁed by the experimental results obtained by other researchers. The transition of planar/cellular interface in solidiﬁcation was also investigated from the standpoint of the diﬀusion controlled solidiﬁcation. [doi:10.2320/matertrans.M2009392]

(Received December 1, 2009; Accepted February 8, 2010; Published April 25, 2010)

Keywords: solute redistribution, upward cellular solidiﬁcation, computer simulation, diﬀusion control, parabolic relation, interface transition

1. Introduction

The solidiﬁcation of a single phase alloy necessitates
diﬀusion of the rejected solute out of the interface into either
or both solid and liquid. The solidiﬁcation of an alloy,
therefore, is related closely to the solute diﬀusion and
considered to be a kind of diﬀusion controlled reaction.
Although solidiﬁcation theories have been stated on the
various conditions of diﬀusion in solid and liquid,1–13) the
diﬀusion controlled solidiﬁcation has not been considered
yet in most of those theories. Since the value of diﬀusion
coeﬃcient in liquid is low, the distance of eﬀective diﬀusion
from its source in a short time is usually restricted to short
ranges14) _{such as the sizes of cell, cellular dendrite and}

dendrite. Accordingly, the present author planned to
inves-tigate the redistribution of solute during the cellular
solidiﬁcation in Al–Cu alloys by means of the computer
simulation. Computer simulation is considered a powerful
tool to clarify the entire process of the diﬀusion controlled
solidiﬁcation. Although the computer analysis of dendritic
solidiﬁcation was carried out already by Brody and
Flem-ings,15) their work seems to be made on the unreasonable
supposition. The present author applies the direct solving
method of diﬀerential equation (DSM) to the diﬀusion in
both solid and liquid. And the advancing distance of the
solid/liquid interface for a minute time is calculated by
equating the amount of rejected solute out of the interface to
the amount of solute which is carried away into solid and
liquid by diﬀusion for the same minute time. Al–Cu alloys
are favorable to the simulation, for the solidus and liquidus
lines are nearly straight and the diﬀusion coeﬃcients in solid
and liquid are known. To avoid the complication of diﬀusion
by liquid motions,13)_{upward solidiﬁcation is supposed. The}

results of simulation are analyzed to show the solute redistribution in solid and liquid during solidiﬁcation, and to induce a general equation which formulates the sell size as a function of cooling rate and the physical properties of the alloy. The validity of thus induced equation is veriﬁed by the experimental data reported by other researchers.10,11) The

transition of planar/cellular interface is also investigated in consideration of the diﬀusion controlled solidiﬁcation.

2. Simulation Technique for Cellular Solidiﬁcation of Al–Cu Alloy

A personal computer is used to simulate the cellular solidiﬁcation of Al–Cu alloys. Liquidus and solidus lines of Al–Cu alloy system are expressed by

CL ¼0:295 ð933TÞ; CS¼kCL

whereCLandCSdenote the concentration (mass%) of solute

copper in liquid and solid at temperatureT(K), respectively, and k the partition coeﬃcient in equilibrium, namely k¼5:65=33¼0:1712. Diﬀusion coeﬃcient of Al–Cu alloy in liquid DL and in solid DS are expressed respectively as

follows.16–18)

DL (cm2/s)¼0:0081 expf38900=ðRTÞg

DS(cm2/s)¼2:3 expf146000=ðRTÞg

whereRexpresses the gas constant, 8.3144 J/(mol K). Figure 1 shows the cross section of a growing lamellar cell whose width is2Lschematically. The cell proceeds upwards along z-axis, and its sideward fattening takes place in x -direction as the temperature falls. Instead of upward proceeding of the cell, temperature at a ﬁxed location in

Fig. 1 Schematic section of a lamellar cell, Al–4 mass%Cu alloy.

*_{Professor Emeritus, Kyushu Institute of Technology}

where m denotes the gradient of liquidus line and m¼ 1=0:295¼ 3:390. IfGis kept constant,dCL=dzbecomes

constant accordingly. Thend2_{C}

L=dz2is equal to 0 in eq. (1).

Accordingly, it is suﬃcient for the simulation to consider
the solute redistribution only along x-direction during
cool-ing. Similar condition of diﬀusion will hold in solid. This
idea that no eﬀective diﬀusion of solute along z-direction
agrees the experimental fact13) _{that no lengthwise }

macro-segregation occurs in the alloy whose solute is heavier than the solvent.

For the conservation of solute, the proceeding of solid/
liquid interface by dx _{requires the diﬀusion of rejected}

soluteðCLCSÞdx out of the interface into both solid and

liquid. This condition is written as follows:

½CLðxÞ CSðxÞdx

¼ dCSðxÞ dx

x DSdt

dCLðxÞ

dx

x

DLdt ð2Þ

whereCSðxÞandCLðxÞexpress themselves to be the functions

of xat temperatureT. Equation (2) shows also that the rate
of solidiﬁcation,dx_{=}_{dt}_{, is controlled by the solute diﬀusion}

in solid and liquid. In order to use the direct solving method
of diﬀerential equation,19)_{DSM, a half cell size}_{L}_{is divided}

byn. The dividing points, or joint, are labeled by number of 0 to n including both ends. Then the distance between the neighboring joints isL¼L=n. The solute concentration at each joint is calculated by DSM, in which Fick’s second law of diﬀusion in solid is developed as follows:

dCSðiÞ ¼dS½CSði1Þ 2CSðiÞ þCSðiþ1Þ

dS¼DSdt=L2¼n2DSdt=L2

where CSðiÞ and dS express the solute concentration at

i-th joint of solid and the dimension-less time increment, respectively. Similar calculation is carried out also in liquid, that is;

dCLðiÞ ¼dL½CLði1Þ 2CLðiÞ þCLðiþ1Þ

dL ¼DLdt=L2¼n2DLdt=L2:

When the location of the interface is halfway between neighboring joints, estimation of the solute concentration at the joint in contact with the interface is necessary. Let p denote the joint number in solid in contact with the interface. Letaexpress the distance between the interface and the joint of number p, andCSI andCLI denoteCS (x) andCL (x),

respectively, as shown in Fig. 2. The solute concentration of jointpin solid is estimated by interpolation as follows:

CSðpÞ ¼CSI ½CSICSðp1Þ a

Lþa ð3Þ

The solute concentration at the supposed joint pin liquid is estimated by extrapolation as follows:

CLðpÞ ¼CLIþ ½CLICLðpþ2Þ a

2La ð4Þ

According to eq. (2), the shift of the interface da¼dx _{is}

calculated as follows:

ðCLICSIÞda¼½CSðpÞ CSðp1ÞDSdt

L

½CLðpþ1Þ CLðpÞDLdt

L ð5Þ

Putting L¼0:01cm, n¼10, dt¼0:05 second, cooling rateV ¼0:5, 1 and 2 K/s, T¼TL and p¼0, calculations

of DSM and eqs. (3) to (5) are started and carried out repeatedly until the eutectic temperatureTE is attained. The

values of L;n and dt are chosen to satisfy the necessary
conditions for DSM, n2_{D}

Ldt=L2<0:5, in consideration of

the experimental results.10,11)_{In every calculation of DSM,}

da;dS and dL are summed up into a, S and L,

respectively. Joint number pis increased by 1 at every time
whenaexceedsL.x _{is numerated as}_{x}_{¼}_{p}_{}_{L}_{þ}_{a}_{, and}

solid fraction fSas fS¼x=L. Solute concentration of solid

and liquid at each joint was printed at the desired stages of solidiﬁcation.

3. Results of Simulation and Considerations

3.1 Relationship between fraction solid f*S* and
temper-atureT

The simulated relations between fraction solid fS and

temperatureTof Al–1, 2 and 4 mass%Cu alloys are shown in
Fig. 3 when cooling rateV¼1K/s. The lines in Fig. 3 are
drawn according to Scheil’s equation2)_{in which no diﬀusion}

in solid and complete diﬀusion in liquid is supposed. The fST relations obtained by simulation shown in Fig. 3

appear in pretty good coincidence with Scheil’s relation for respective alloys. It is realized that the higher the copper content of the alloy, the wider becomes the liquid groove between the neighboring solid cells.

The depth of liquid groove, however, becomes ðTL

[image:2.595.342.510.68.202.2]found that only a little change of fSTrelation occurs when

the calculation of the ﬁrst term in right side of eq. (5) is
omitted. For example, the ﬁrst term in the right of eq. (5)
is 6:13108_{mass%/(cm}2_{}_{s), while the second is} _{6}_{:}_{82}_{}
105_{mass%/(cm}2_{}_{s) when} _{C}

0¼4mass%Cu, V ¼1K/s

and fS¼0:5. The ratio of the two becomes9:0104. This

is the reason why the ﬁrst term in the right of eq. (5) is negligible.

Figure 4 shows the eﬀect of cooling rate on the simulated fST relation of Al–4 mass%Cu alloy in comparison with

the relations in equilibrium and of Scheil. Figure 4 shows almost no eﬀect of cooling rate on the fST relation.

Figure 4 also shows that the temperature of simulatedfST

relation lowers away from the equilibrium after the value of fS exceeds about 0.5. This super-cooling may be the

driving force for the second arms of cellular dendrite to grow and the super-cooling is somewhat decreased to approach equilibrium.

3.2 Solute redistribution in solid and liquid during solidiﬁcation

Figure 5 shows the solute distribution in solid and liquid at every intervals of 0.2 fraction solid during the solidiﬁcation of Al–4 mass%Cu alloy. The solute concentration at each joint in liquid changes large with the progressive

solid-iﬁcation, while the solute concentration at each joint in solid changes only a little during the solidiﬁcation. Therefore, the change in solute concentration in solid after the passage of interface is not drawn in Fig. 5 to avoid confusion.

The curves of solute distribution in liquid shown in Fig. 5 are characterized by the gentle slope toward cell boundary, and by the parallel shift between the curves.

In order to examine the solute distribution in liquid more precisely, CLðiÞ CLðnÞ of i-th joint is plotted against

ð1i=nÞ2 at every intervals of 0.2 fraction solid in Fig. 6. Figure 6 indicates that the distribution curves are parabola whose bottom zeniths lie at the cell boundaryx¼L, and that the diﬀerence in concentrationCLðiÞ CLðnÞis proportional to the cooling rate. The parabolic solute distribution is written in general as follows;

CLðxÞ ¼CLðnÞ þbð1x=LÞ2 ð6Þ

where b expresses a constant. The second order derivative of eq. (6) aboutxgives the following equation.

d2CLðxÞ

dx2 ¼ 2b

L2 ð7Þ

Fig. 3 Simulated relation between fraction solidfSand temperatureTin comparison with that of expected from Scheil’s equation for Al–1, 2 and 4 mass%Cu alloys.

Fig. 4 Eﬀect of cooling rate on thefSTrelation of Al–4 mass%Cu alloy.

Fig. 5 Distribution of copper concentration in solid and liquid at several stages of solidiﬁcation of Al–4 mass%Cu alloy.

[image:3.595.68.270.69.234.2] [image:3.595.324.526.71.240.2] [image:3.595.323.528.288.470.2] [image:3.595.69.271.289.453.2]Consequently, eq. (6) can be rewritten as follows:

CLðxÞ ¼CLðnÞ þ

V 2mDL

ðLxÞ2 ð11Þ

Equation (11) shows thatCLðxÞ CLðnÞbecomes zero when

DLis inﬁnity, that is, when the diﬀusion in liquid is complete.

This condition of diﬀusion in liquid agrees quite well with that of Scheil. That is, the complete mixing in liquid supposed by Scheil is taken as an extreme case of the diﬀusion controlled solidiﬁcation.

Derivative of eq. (11) is written as follows:

dCLðxÞ

dx ¼

V mDL

ðLxÞ ð12Þ

Since the diﬀusion in solid is negligible, eq. (2) can be rewritten as follows by using eq. (12):

ðCLCSÞdx¼

V m ðLx

_{Þ}_{dt} _{ð13Þ}

Since x_{=}_{L}_{¼} _{f}

S and Vdt=m¼dCL at the interface, the

following equation is given.

ð1kÞCLd fS¼ ð1fSÞdCL ð14Þ

Equation (14) is quite the same as Sheil’s equation. This is the reason why the simulatedfSTrelation coincides pretty

well with that of Scheil in lamellar cells whose size 2L is small enough to cause the parabolic solute distribution in liquid in a short time. In other words, Scheil’s equation is approximately applicable to the lamellar cell forming solid-iﬁcation of actual alloys whose diﬀusion is incomplete.

To examine the solute distribution in solid more precisely, an example of the simulated values of concentration at solid joint at several stages of solidiﬁcation is shown in Table 1. The concentration at each solid joint calculated from Scheil’s relation is also shown in Table 1. Table 1 shows that the simulatedCSof the interface at a ﬁxed location diﬀers a little

from that of Scheil’s relation essentially, because of the incomplete mixing of solute in liquid. Table 1 shows also a little more change in CS caused by the diﬀusion after

the passage of interface. The former diﬀerence in CS is

considered to increase as the cooling rate increases, because the mixing in liquid becomes more incomplete. The latter diﬀerence inCSis considered to decrease as the cooling rate

increases on the contrary. However, the cell width L is dependent on the cooling rateV, that is, the parabolic relation of cellular solidiﬁcation is dominant, which will be stated later.

Under the parabolic relation between the cell size and cooling rate, the redistribution of solute in relative location of solid was found not to vary during the solidiﬁcation, however the cooling rate of an alloy may change.

Figure 7 shows the peculiar solute distributions of three alloys with diﬀerent solute content at the time when eutectic temperature is reached (open circles), together with that of Scheil’s relation. Figure 7 shows that the simulated solute concentration at each joint diﬀers only a little from that of Scheil.

When the temperature decreases below eutectic temper-ature, CuAl2in eutectic begins to dissolve into the primary

solid solution and homogenizing diﬀusion of solute will take place in the cell. However, the solubility limit as well as the diﬀusion coeﬃcient in solid decrease with lowering of temperature. Therefore, the change of solute concentration in the solid cell below eutectic temperature is considered to be very few. That is, the solute distribution in the cell after the solidiﬁcation can be approximated by the integrated relation of Scheil’s equation, eq. (14), as follows:

CS¼kC0ð1fSÞk1

Flemings stated that the solute distribution in dendritic solid is expressed as follows:20)

CS¼kC0 1 fS

1þk

k1

; ¼DStF

L2 ð15Þ

[image:4.595.319.533.124.399.2]wheretFrepresents local solidiﬁcation time, that is the time

required to cool from liquidus to solidus. Kurz and Fisher showed the mass balance equation as follows:21)

CL=C0¼ ½1fSð12kÞ

¼ ðk1Þ=ð12kÞ ð16Þ

In the present simulation,dtwas summed up intotFuntil

eutectic temperature is attained. The result of the simulation was tF¼96:75s, S¼ðn2DSdt=L2Þ ¼n2DSAvtF=L2¼

0:448, L¼ðn2DLdt=L2Þ ¼n2DLAvtF=L2 ¼3631 when

V ¼1K/s, L¼0:01cm and n¼10. Therefore, DSAv¼

4:63109cm2/s. When the temperature range of solid-iﬁcation is expressed by T, T ¼TLTE¼96:75K.

Since tF¼T=V and the value ofVL2 is numerated to be

6:26104_{Kcm}2_{/s for lamellar cell of Al–4 mass%Cu}

alloy as will be seen later, tF=L2¼1:55105s/cm2 and

¼DSAvT=VL2¼7:16104. Then the value of is

very small in comparison with unity. Accordingly, both eq. (15) and eq. (16) turn to Scheil’s equation. Therefore, it contradicts neither eq. (15) nor (16) that Scheil’s equation is approximately applicable to the result of the present simulation.

Figure 8 shows the simulated solute distribution in solid at several stages of solidiﬁcation on the assumption that L¼0:02cm, V ¼ 1K/s, DS¼106cm2/s (¼0:2419).

Figure 8 looks like the work by Brody and Flemings15)at ﬁrst sight. But their work seems to be made on the inadequate assumption. They supposed the complete mixing in liquid, which they misunderstood as no diﬀusion in liquid.

They considered, therefore, the whole amount of solute rejected out of the interface had to be carried oﬀ by the solid diﬀusion and calculated as tF=L2¼3:3108s/cm2. And

they made the work by usingtF=L2¼3:3108s/cm2which

is several thousands times larger than the real one. Since most of the solute is carried oﬀ by the liquid diﬀusion actually as described above, their assumption is inadequate. In addition, the solute concentration of solid which solidiﬁes at the start has to be kC0¼0:77mass%Cu as shown by eqs. (15) and

(16), however the value of or tF=L2 may change. But

their ﬁgure shows 0.61 mass%Cu. Perhaps, they would miscalculate as k¼4:5=33¼0:1364 and kC0¼0:1364 4:5¼0:6138mass%Cu.

Broken lines in Fig. 8 show solute distributions of solid calculated by eq. (15) using ¼0:2419 and by Scheil’s relation. The broken line of eq. (15) indicates the approx-imate solute concentration in solid at a given relative location in the cell when the interface passes over, but it does not show the solute distribution at or after the passage of the interface. Equation (16) shows almost similar pattern of the solute distribution curve to that of eq. (15).

Figure 9 shows the solute distributions in solid with varied values ofDSwhen eutectic temperature is just attained. The

value ofDSis increased much to get a comparable value of

to unity instead of thetF=L2. The ﬁgure shows that the larger

the diﬀusion coeﬃcient of solid, the more gentle becomes the
slope of solute distribution. Although the solidiﬁcation in
equilibrium is expected when ¼0:5 from eq. (16),21)_{the}

solute distribution d (¼0:4839) in Fig. 9 seems still far from the equilibrium or homogeneous solute distribution.

3.3 Parabolic law of cellular solidiﬁcation

The processes of cellular solidiﬁcation with varied cooling rate are shown in Fig. 10, in which dimension-less time DLAvt=L2 is taken as abscissa. DLAvt=L2 is numerated by

elimination ofn2fromn2DLAvt=L2as follows:

DLAvt=L2¼ðn2DLt=L2Þ=n2¼ðdÞ=n2¼=n2

It is natural that the dimension-less time required to attain a deﬁnite temperature fall (a) and a deﬁnite fraction solid (b) is inversely proportional to the cooling rate. The slopes of the solidiﬁcation curves shown in Fig. 10(b) are written as follows:

L2_{d f}

S

DLdt

¼VL 2

DL

d fS

Vdt¼ VL2

DL

d fS

dT

Use of eq. (14) givesd fS=dTas follows:

d fS

dT ¼ dCL

dT d fS

dCL

¼ 1fS

mðk1ÞCL

Combination of above two equations results in following equation:

L2d fS

DLdt

¼ VL

2_{ð1}_{}_{f}

SÞ

mðk1ÞCLDL

ð17Þ

Fig. 8 Solid lines in order toward top show the solute distributions in solid at fS¼0:1, 0.3, 0.5, 0.7, 0.9 and 0.95, respectively, on the assumption

DS¼106cm2/s, while broken lines show Scheil’s relation and eq. (15).

[image:5.595.70.268.70.233.2] [image:5.595.325.526.72.233.2]The solid line in Fig. 11 shows the dimension-less rate of solidiﬁcation calculated by using eq. (17) for Al–4 mass%Cu alloy, and the plots are the results of simulation. Details about the drawing of Fig. 11 are as follows.

The values of right side of eq. (17) are numerated to be 0.178, 0.143, 0.117, 0.094, 0.072 and so forth at fS¼0, 0.1,

0.2, 0.3, 0.4 and so forth, respectively by the use ofCLandDL

at each stage when V ¼1K/s, Al–4 mass%Cu alloy. Solid
line is made using these data. In the simulation of the same
conditions, the required=n2_{or}_{D}

LAvt=L2to attain fS¼0:1,

0.2, 0.3, 0.4 and so forth becomes 0.8928, 1.6031, 2.4702,
3.6090 and so forth, respectively. Use of these data gives
L2_{d f}

S=DLdt¼0:112, 0.141, 0.115, 0.088 and so forth at

fS¼0:05, 0.15, 0.25, 0.35 and so forth in average,

respectively. Simulations of the soliodiﬁcation with V¼ 0:5 and 2.0 K/s are carried out similarly. These data are plotted in Fig. 11.

Although the rate of solidiﬁcation at the start calculated by using eq. (17) is 0.178 for the alloy, the simulated rates appear about 25% decrease as shown in Fig. 11 and also in Fig. 10. The misﬁt is partly attributable to the unskilled

cellular solidiﬁcation is a kind of diﬀusion controlled reaction showing parabolic relation betweenV andL.

Taking into account of the decrease in solidiﬁcation rate in early stage, eq. (18) gives the following;

0:75V0L2¼mðk1ÞC0DL ð19Þ

where V0 denotes the cooling rate at the start, and C0 the

original solute content of the alloy.

So far, the lamellar cell forming solidiﬁcation is supposed.
In the experiments by other researchers,10–12) _{however,}

crossed cells were observed in columnar crystals. Then two-dimensional solute diﬀusion should be considered during solidiﬁcation. However, the cellular solidiﬁcation is considered to progress by fattening of the crosses, which is expressed as follows:

fS¼1 ðLxÞ2=L2 ¼2x=L ðx=LÞ2

In the early stage of solidiﬁcation, the second term in the
right (x_{=}_{L}_{Þ}2 _{is negligible. Accordingly, the rate of the}

crossed cell forming solidiﬁcation in early stage is estimated to be twice as fast as that of the lamellar cell forming solidiﬁcation. That is,

[image:6.595.68.269.70.244.2]1:5V0L2¼mðk1ÞC0DL: ð20Þ

Figure 12 shows plots of the crossed cell size L against

½mðk1ÞC0=V01=2 for Al–Cu,10) Al–Si10) and Cu–Zn11)

alloys obtained experimentally by other researchers. Two straight lines express L vs.½mðk1ÞC0DL=V01=2 relations

calculated by the use of eq. (19) and eq. (20) on the supposition that DL¼5105cm2/s, which may be

roughly admitted for the low temperature dependence of DL. Experimental results shown in Fig. 12 appear roughly in

good coincidence with the calculated relation in alloys which have their ownmandk.

Ibarakiet al.derived a theoretical equation for the cellular
solidiﬁcation with crossed cells10)_{as follows:}

L¼a0

½mðk1ÞDL1=2

k ½C0=V0

1=2 _{ð21Þ}

where a0 denoted a constant. Equation (21) indicates that

the cell size Lis proportional to the square root of C0=V0,

which was proved by their experimental data of Al–Cu and Al–Si alloys.10)However, eq. (21) contains a unknown constant, a0, and, therefore, it is unable to prove the

[image:6.595.68.270.309.471.2]experimental results quantitatively. Sugiyamaet al.12)carried out similar experiments on Cu–Sn alloys and derived an experimental equation to explain the results as follows: Fig. 10 Plots of temperature drop (a) and fraction solidfS(b) as a function

of dimension-less time of solidiﬁcationDLAvt=L2for Al–4 mass%Cu alloy in varied cooling rates.

L¼1:1 ðC0=V0Þ1=2 ð22Þ

But V0 is taken as the ratio of the diﬀerence between the

casting temperature and liquidus temperature by the time passed in their experiment. Therefore, eq. (22) is not a general equation for the cellular solidiﬁcation. Donaghey and Tiller22)calculated the size of lamellar cell on the assumption of the simpliﬁed morphology of liquid groove between cells. The result was in accord with what was expected in a special condition.

Consequently, eqs. (18), (19) and (20) seem superior to other theories quoted above, for these equations are in good quantitative coincidence with the experimental results with-out containing any unknown variable.

4. Transition of Planar/Cellular Interface

B. Chalmers introduced the constitutional super-cooling to explain the transition of planar/cellular interface as follows:23)

G R ¼

mC0ð1kÞ kDL

ð23Þ

Tiller stated an equation on the supposition of the constitutional super-cooling caused by the partial solute mixing in liquid under constrained solidiﬁcation as fol-lows:24)

G

R ¼

mCLðiÞð1kÞ

DL

ð24Þ

where CLðiÞ denoted solute concentration in liquid at the

interface.

However, when the diﬀusion controlled solidiﬁcation with
planar interface perpendicular toz-axis is considered, another
criterion for the transition appears. Neglecting the ﬁrst term
in the right side of eq. (2) and putting the growth rate
R¼dz_{=}_{dt}_{, eq. (2) along}_{z}_{-axis turns to}

R¼ dCL dz

z

DL

CLðzÞð1kÞ

The concentration gradient of liquid in contact with the

solid-liquid interface is converted to the gradient of corre-sponding liquidus temperatureGCas follows:

GC¼

dT

dz

z

¼ dT

dCLðzÞ

z

dCLðzÞ

dz

x

¼m dCLðzÞ dz

z

Hence, the combination of above two equations gives the following equation:

GC

R ¼

mCLðzÞð1kÞ

DL

CLðzÞ increases as the solidiﬁcation progresses and so

doesGC=R. Supposing the upward solidiﬁcation in a furnace

with its ﬁxed temperature gradientG, the solidiﬁcation with planar interface will become unstable when GC exceedsG,

and protrusions of the interface will grow into the liquid, and cellular interface will be formed. And the solute diﬀusion in liquid along z-direction will change to the diﬀusion along x-direction at the same time. That is, the transition of planar/ cellular interface is expressed as follows:

G

R ¼

mCLðzÞð1kÞ

DL

ð25Þ

Equation (25) is quite the same as eq. (24). The coincidence between the two is convincible when the partial solute mixing model by Tiller is considered to play the role of the parabolic solute distribution in liquid.

The transition of ‘‘No Cell/Cell’’ interface in Pb–Sn alloys
stated by Rutter25) _{shows that the ratio of} _{C}

0 to G=R is
3:2105_{mass%cm}2_{/Ks. Since}_{m}_{¼ 2}_{:}_{32}_{K/mass% and}
k¼0:31, DL is numerated to be 5:1105cm2/s by

eq. (25) and1:7104_{cm}2_{/s by eq. (23). The former value}

of DL seems more plausible than the latter, although the

exact value ofDL for the alloy is not known.

Equation (25) indicates also the condition for the forma-tion of cellular structure. For example, the right term of eq. (25) is from about5104to5105Ks/cm2for Al–Cu alloys of low solute content, while the left term of eq. (25) in the experiment done by Ibaraki et al. was about 100 to 400 Ks/cm2. The smallness of the latter in comparison with the former seems to be the reason why the cellular structure was formed in their experiment.

5. Conclusion

In order to study the solute redistribution in solid and liquid during the upward cellular solidiﬁcation of Al–Cu alloy, computer simulation was carried out by using the direct solving method under the supposition of the diﬀusion controlled solidiﬁcation. The simulated results were analyzed and summarized as follows:

[image:7.595.69.269.69.236.2](1) The solute distribution in liquid ahead of the solid-liquid interface was found parabola whose bottom zenith lies at cell boundary. Hence, the increasing rate of solute concentration becomes equal everywhere in liquid during the solidiﬁcation on linear cooling.

reaction.

(6) Thus derived formula was veriﬁed by the experimental cell sizes obtained by other researchers in Al–Cu, Al–Si and Cu–Zn alloys.

(7) The transition of planar/cellular interface was inves-tigated in consideration of the diﬀusion controlled solid-iﬁcation and a new condition for the transition was formulated.

REFERENCES

1) B. Chalmers:Principles of Solidiﬁcation, (Jhon Wiley & Sons Inc. New York) (1964) pp. 126–185.

2) E. Scheil: Z. Metallk.34(1942) 70. 3) W. G. Pfann: Trans. AIME236(1966) 615.

4) M. C. Flemings:Solidiﬁcation Processing, (Trans Tech Publications, Switzerland) (1986) p. 31.

5) W. Kurz and D. J. Fisher:Fundamentals of Solidiﬁcation, (Trans Tech Publications Ltd.) (1986) p. 121.

(1963) p. 1.

15) H. D. Brody and F. C. Flemings: Trans. AIME236(1966) 615. 16) K. Uemura: Tetsu-to-Hagane25(1939) 24.

17) T. Owadano, N. Ofuchi and K. Yusa: Report of Kyushu Inst. of Technology, Technology Branch22(1971) 45–50.

18) R. M. Barrer: Proc. Soc.52(940) 58.

19) G. D. Smith: Numerical solution of Partial Diﬀerential Equations, (Oxford University Press, 1965) (Translated by Y. Fujikawa into Japanese, Saiensu Co. Ltd., 1971) pp. 9–56.

20) M. C. Flemings:Solidiﬁcation Processing, (Trans Tech Publications, Switzerland) (1986) p. 134.

21) W. Kurz and D. J. Fisher:Fundamentalsof Solidiﬁcation, (Trans. Tech. Publications Ltd.) (1986) p. 230.

22) L. F. Donaghey and W. A. Tiller:The Solidiﬁcation of Metals, (Iron and Steel Inst. London, 1967) pp. 87–92.

23) B. Chalmers:Principles of Solidiﬁcation, (Jhon Wiley & Sons Inc. New York, 1964) pp. 154–163.

24) W. A. Tiller:The Science of Crystallization, (Cambridge University Press, 1991) p. 246.